Synthesis and Characterize of Bi0.6Sb1.4Te3 Nano-particles from Long Pulsed Laser Ablation
Long pulsed laser ablation was applied to synthesis Bi0.6Sb1.4Te3 nano-sized particles of corresponding bulk target in argon environment. Normally, short laser pulses, nanosecond or less, have been used. This work involves with an economical technique involving a Nd:YAG laser working at 1064 nm and millisecond long pulses. System operating parameters including laser frequency (1 Hz), pulse duration variation (1, 3, 5 msec) and target speed at 3000 rpm (2.2 m sec-1) were held constant. The particles produced by laser ablation have been characterized by scanning electron microscopy and X-ray diffraction for the morphology and the crystallographic structure of the nano-particles. The experiment shows that the particles were produced in the form of aggregates of primary particle in the nanometer size range between 20 and 120 nm depend on irradiation laser fluence. This technique can prepare mass production of nano-particles in a very short time when compare to femtosecond or nanosecond laser.
Received: February 08, 2011;
Accepted: April 11, 2011;
Published: December 16, 2011
Several techniques for preparation of different nanoparticles such as hydrothermal
method for Al doped ZnO (Suliman and Tang, 2007), reduction
and microwave heating for Au (Mohamad et al., 2010)
while anode support system for Cu2O (Abdulkarem
et al., 2007) and using of plant to biosynthesis of silver nanoparticles
had been reported recently. In this work, a new method of long pulsed laser
ablation technique has been employed in the preparation of Bi0.6Sb1.4Te3
The modern history of laser ablation begins with the discovery of the ruby
laser by Maiman in 1960 and the first published account of ablation is the abstract
of a talk given by F. Breech and L. Cross at the International Conference on
Spectroscopy at the University of Maryland in June 1962 (Miller,
1993). The Pulse Laser Ablation (PLA) is a process for removing material
from a solid surface by irradiating it with a laser beam. The PLA can apply
to many applications such as laser cleaning of a medieval wooden panel chamber
(Wiedemanna et al., 2000), etching of GaN film
by UV laser at 266 nm (Zhang et al., 1998), ablation
of ZrO2 and CeO2 by different laser pulse duration and
thin films deposition by Nd:YAG laser at 1064, 532 and 355 nm, an ArF excimer
laser at 248 nm and a Nd:glass laser at 529 nm (Guidoni
et al., 2000), annealing treatment of Bi (Pb)-Sr-Ca-O thin film (Jannah
et al., 2009) and preparation of conventional thermoelectric nanopowders
in water by Nd:YAG laser at 532 nm (Kosalathip et al.,
Generally, PLA use short laser pulses between femtosecond to nanosecond with
low speed moving target so they are expensive laser mechanism (Rudolph
et al., 1999). The femtosecond laser was used to prepare metal nano-particles.
Tsuji et al. (2003) presented the silver nano-particles
synthesize by femtosecond laser ablation when increased laser wavelength influence
particle size increasing. Our study a new technique for synthesis allow nano-particles
by long laser pulses in order of microsecond while the target is moving at high
speed under argon pressure. By the target is a thermoelectric material of bismuth
antimony telluride. Thermoelectric devices are the possible candidates to generate
direct electricity from the available thermal radiation as well as other heat
sources and have many types of compound on used temperature. Bismuth antimony
telluride is a famous thermoelectric material on room-temperature. The efficiency
of a thermoelectric material application is determined by the dimensionless
figure of merit, defined as: ZT = S2σT/k. Where S, σ, k
and T are the Seebeck coefficient, electrical conductivity, thermal conductivity
and absolute temperature, respectively. Hostler et al.
(2008) study the particle-size influential to thermoelectric properties.
That work was show the technique of improvident thermoelectric efficiency of
bismuth bulk by used low-dimensional structures a pellet composed of bismuth
nano-particles. In the aim of this research is to use the alternative low cost
to improve morphology, size and crystal structure for thermoelectric material.
MATERIALS AND METHODS
The target materials were compound of Bi, Sb and Te in Bi0.6Sb1.4Te3
stoichiometry and were 15 mm in diameter and 3 mm in height which were prepared
as described by hot-pressing method (Kumpeerapun et al.,
2006). They were cleaned with acetone in an ultrasonic cleaner and mounted
on a high speed motor in argon chamber at atmospheric pressure and were radiated
at normal incident using convex lens of focal length f = 50 mm at 1064 nm (Fig.
1). The speed of the motor has been fixed at 3000 rpm or 2.20 m sec-1
(at 15 mm diameter). The pulse duration of the laser beam has been varied from
1 to 10 msec. The output energy is 0.5 J/pulse. The laser used for this work
is a pulsed Nd:YAG laser working at 1064 nm. First, a heat effect zone at the
surface of the target after interacted by laser pulses when difference pulse
durations ranging 1 ms to 5 ms and high moving target speed at 2.20 m sec-1
was studied. After obtained and characterized the morphology, the particle size
and target surface were analyzed by using a Scanning Electron Microscope (SEM).
The crystallographic structural of the obtained nanoparticles were determined
by X-Ray Diffraction (XRD). In this case, the nano-particles in the form of
spherical in chains which flown away from the target were collected at the 20
mm in diameter of cylinder substrate. A thick black layer of nanopowder was
obtained for XRD measurements.
|| Diagram of experiment setting
RESULTS AND DISCUSSION
Laser interaction: Initially, the effects of pulse duration of a laser
beam shot on non-moving target and on high speed of 3000 rpm (2.20 m sec-1)
were investigated by varying the pulse durations between 1 to 5 msec.
||SEM images of heat-zone surface on non-moving target, (a)
1 msec, (b) 3 msec and (c) 5 msec pulse durations
|| SEM images of heat-zone surface on moving target at 2.20
m sec-1, (a) 1 msec, (b) 3 msec and (c) 5 msec pulse durations
||Cross sectional SEM images of non-moving target, (a) 1 msec,
(b) 3 msec and (c) 5 msec pulse durations
||Cross sectional SEM images of moving target at 2.20 m sec-1,
(a) 1 msec, (b) 3 msec and (c) 5 msec pulse durations
Figure 2 and 3 show the surface of heat-zone
for non-moving and moving targets with the pulse durations were set at 1, 3
and 5 msec, respectively. Figure 2 shows the top view of melting
area by single pulse laser interaction on non-moving target. The diameters of
melting zone increases from 0.93, 1.16 and 1.30 mm and laser fluences increases
from 7.36, 18.92 and 24.11 J cm-2 as the pulse durations increase
from about 1, 3 and 5 msec, respectively. Figures 4 are cross
section of non-moving conditions. The melting depth-hilliness distances increases
from 40, 60 and 73 μm as the pulse duration increase from about 1, 3 and
5 ms, respectively. The laser beam interacts to surface, the target is melting
and then inflating because of its cooling down. When the higher energy
used, the melting and inflating zones are broad compares to the lower energy.
Figure 5 shows cross section of moving conditions, the melting
depth distances about 40 μm at every conditions of pulse duration due to
the moving target decrease laser fluences.
Nanoparticles morphological: Initially, the effects of one shot from
the laser beam on the target surface while the target was moving at the high
speed of 3000 rpm (2.20 m sec-1) and non-moving condition when varying
the pulse durations between 1 to 5 msec were studied. Figure 2
and 3 show that the heat-zone on surface of non-moving target
and cross section by setting pulse duration at 1, 3 and 5 msec, respectively.
The SEM image in Fig. 6a-c show the appearance
and particle sizes obtained from the difference pulse durations at the same
target speed (2.20 m sec-1). The results shown the particle size
distribution obtained from lower fluence is smaller than the higher fluence
and the particle size mostly are in range of 10 to 120 nm as in Figure
6d. The average size of outcome nanoparticles 42.24, 48.96 and 55.70 nm
are obtain from 1, 3 and 5 msec pulse durations, respectively.
For the morphology, the short colony and amount of nanoparticles was obtained
from 1 ms laser pulse duration while longer pulse durations, 3 and 5 ms, give
the more amount and longer chain of nanoparticles, the accumulation are rarely
occur (Fig. 6a-c).
When the longer pulse duration of the laser beam was applied (Fig.
2-5), the larger area and deeper heat effect zone was
created. This shows that more particles and larger particles could be formed
from the larger melt volume due to the longer pulse duration of laser beam.
The deeper of the heat effect zone near the center could create the larger size
of the particles. The smaller size of the particles could come from the melting
area which is far away from the center of the melting zone. This means that
the thin layer of the melting zone created the formation of the smaller size
of nanoparticles while the thick layer of the melting zone created the larger
size of nanoparticles Fig. 6d could be used to support this
concept. Other than that the longer chain of the groups of nanoparticles were
also created due to larger volume of the melting target when the longer pulse
duration of laser beam was applied.
||SEM images of Bi0.6Sb1.4Te3
nanoparticles were prepared when difference pulse durations at (a) 1 msec,
(b) 3 msec and (c) 5 msec and (d) size distribution
||Crystallographic structure of (a) Bi0.6Sb1.4Te3
nanoparticles, (b) Bi0.6Sb1.4Te3 target
and (c) JCPDS file number 49-1713
The pulse duration also effecting the particle size, the used of shorter pulse
duration has been shown the produce smaller particle size as also had been reported
in the synthesizing of thermoelectric nanopowders (<35 nm) with pulse duration
of 7 ns (Kosalathip et al., 2008).
Nanoparticles crystal structural: The crystal structures of target and
nanoparticles from 5 ms pulse duration were used to characterize by XRD (Fig.
7). The XRD pattern present the dominate peak at 2θ = 28°. This
peak could neither be attributed to one of simple elements, Bi, Te, or Sb, nor
to any known compound indexed in the JCPDS files. The unknown peak also appeared
similar to the work of Kosalathip et al. (2008)
who prepared their nanoparticles in liquid medium. The XRD pattern obtained
were correspond to JCPDS 49-1713 of bismuth antimony telluride in rhombohedra
structure and showed (0 1 5), (1 0 10), (1 1 0) and (0 0 15) reflection.
This work shows a simple and low cost method to synthesize nanoparticles of complex composition, obtained from Bi0.6Sb1.4Te3 target by long laser pulses in argon atmospheric. This method uses decreasing laser fluence technique and takes a short time preparation and no further treatment necessary. The cost of millisecond pulse laser is much cheaper than the nanosecond pulse laser. There are no needs to use a high cost vacuum system or liquid medium container. The particle morphology and size were changed by difference pulse duration. The particle preparing process uses long laser pulse cause melting target and spread by rotate speed.
The authors are thankful to Human Resource Development in Science Project (Science Achievement Scholarship of Thailand, SAST).
1: Suliman, A.E. and Y. Tang, 2007. Preparation and properties of Zinc oxide doped with aluminum nanostructured thin film. J. Applied Sci., 7: 314-316.
CrossRef | Direct Link |
2: Mohamad, M.F., K.S.N. Kamarudin, N.N.F.N.M. Fathilah and M.S. Mohamed, 2010. Effects of PVP concentration on the formation of size and shape of gold (Au) nanoparticles for mercury adsorption. J. Applied Sci., 10: 3374-3378.
3: Abdulkarem, A., E.A. Ammar, Y. Ying and L.J. Lin, 2007. Preparation of Cu2O from TiO2 and CTAB using the anode support system. J. Applied Sci., 7: 4674-4678.
CrossRef | Direct Link |
4: Miller, J.C., 1993. A brief history of laser ablation. AIP Conf. Proc., 288: 619-622.
5: Wiedemanna, G., M. Schulzb, J. Hauptmanna, H.G. Kusch , S. Mullera, M. Panznera and H. Wusta, 2000. Laser cleaning applied in the restoration of a medieval wooden panel chamber at Pirna. J. Cult. Heritage, 1: 247-258.
6: Zhang, J., K. Sugioka, S. Wada, H. Tashiro and K. Midorikawa, 1998. Study on high-speed melting depth etching of GaN film by UV laser ablation. J. Cryst. Growth, 189-190: 725-729.
7: Guidoni, A.G., C. Flaminia, F. Varsanoa, M. Riccic, R. Teghilc, V. Marottab and T.M.D. Palma, 2000. Ablation of transition metal oxides by different laser pulse duration and thin films deposition. Applied Surf. Sci., 154-155: 467-472.
8: Jannah, A.N., S.A. Halim and H. Abdullah, 2009. Annealing treatment of Bi (Pb)-Sr-Ca-Cu-O Thin Films on MgO by pulsed laser deposition. J. Applied Sci., 9: 2190-2193.
CrossRef | Direct Link |
9: Kosalathip, V., A. Dauscher, B. Lenoir, S. Migot and T. Kumpeerapun, 2008. Preparation of conventional thermoelectric nanopowders by pulsed laser fracture in water: Application to the fabrication of a pn hetero-junction. Applied phys. A Mater. Sci. Process., 93: 235-240.
10: Rudolph, P., J. Bonse, J. Kruger and W. Kautek, 1999. Femtosecond and nanosecond-pulse laser ablation of bariumalumoborosilicate glass. Applied phys. A Mater. Sci. Process., 69: 763-766.
Direct Link |
11: Tsuji, T., T. Kakita and M. Tsuji, 2003. Preparation of nano-size particles of silver with femtosecond laser ablation in water. Applied Surf. Sci., 206: 314-320.
12: Hostler, S.R., Y.Q. Qu, M.T. Demko, A.R. Abramson, X. Qiu and C. Burda, 2008. Thermoelectric properties of pressed bismuth nanoparticles. Superlattices Microstruct., 43: 195-207.
13: Kumpeerapun, T., H. Scherrer, J. Khedari, J. Hirunlabh and S. Weber et al., 2006. Performance of low-cost thermoelectric modules fabricated from hot pressing and cold pressing material. Proceedings of the 25th International Thermoelectrics Conference, Aug. 6-10, Vienna, Austria, pp: 136-140.